Serving the Grease Industry Since 1933 - VOL. 83, NO. 2, MAY/JUNE 2019
-1VOLUME 83, NUMBER 2
In this issue:â€Ś
4 Exploratory Studies on Borate Esters as Dropping Point Enhancers 14 A Novel Testing Approach to Validating Automotive Lubricant Performance in Fretting Conditions 28 The Cost of Compromise: Wind Turbine Main Shaft Grease Lubrication Engineering Study 46 An Interview with Mr. Durgesh Sanjivrao Chandavarkar 53 Fundamental study of the initial agglomeration of lithium soap thickener in lubricating oil
VICE PRESIDENT: Jim Hunt Tiarco Chemical 1300 Tiarco Drive Dalton, GA 30720
SECRETARY: Dr. Anoop Kumar Chevron Lubricants 100 Chevron Way Room 71-7334 Richmond, CA 94801
TREASURER: Wayne Mackwood Lanxess Corporation 565 Coronation Dr West Hill, Ontario, M1E 2K3 Canada EXECUTIVE DIRECTOR: Crystal O’Halloran, MBA, CAE NLGI International Headquarters 118 N Conistor Street, Suite B-281 Liberty, MO 64068
PAST-PRES./ADVISORY: David Como Molykote P.O. Box 0994 Midland, MI 48686
DIRECTORS Jeff St. Aubin AXEL Royal, LLC PO Box 3308 Tulsa, OK 74101
Dwaine (Greg) Morris Shell Lubricants 526 S. Johnson Drive Odessa, MO 64076
Barbara Bellanti Battenfeld Grease & Oil Corp. of NY P.O. Box 728 • 1174 Erie Ave. N. Tonawanda, NY 14120
George Sandor Livent Corporation 2801 Yorkmont Rd., Suite 300 Charlotte, NC 28208
Richard Burkhalter Covenant Engineering Services 140 Corporate Place Branson, MO 65616
John Sander Lubrication Engineers, Inc. P.O. Box 16447 Wichita, KS 67216
Willie Carter Calumet Branded Products, LLC One Purple Lane Porter, TX 77365
Tom Schroeder Axel Americas, LLC P.O. Box 12337 Kansas City, MO 64116
Chuck Coe Grease Technology Solutions LLC 35386 Greyfriar Dr Round Hill, VA 20141
Simona Shafto Koehler Instrument Co. 85 Corporate Dr. Holtsville, NY 11716
Maureen Hunter King Industries, Inc. Science Road Norwalk, CT 06852
Thomas W. Steib The Elco Corporation 1000 Belt Line Street Cleveland, OH 44109
Tyler Jark Lubricating Specialties Co. 8015 Paramount Blvd. Pico Rivera, CA 90660 Jay Coleman Ergon, Inc. P.O. Box 1639 Jackson, MS 39215 Matthew McGinnis Daubert Chemical Company 4700 S. Central Ave. Chicago, IL 60638
OFFICERS PRESIDENT: Joe Kaperick Afton Chemical Corporation 500 Spring St. Richmond, VA 23218-2158
Serving the Grease Industry Since 1933 - VOL. 83, NO. 2, MAY/JUNE 2019
Exploratory Studies on Borate Esters as Dropping Point Enhancers Vennampalli M., Pokhriyal N.K., Bansal V. R., Saxena D. and Ramakumar S.S.V Indian Oil Corporation Limited, R&D Centre, Sector 13, Faridabad, India
A Novel Testing Approach to Validating Automotive Lubricant Performance in Fretting Conditions Dr. Jason T. Galary
The Cost of Compromise: Wind Turbine Main Shaft Grease Lubrication Engineering Study Edward Worthington and Dwaine Morris Shell Product Technology Hamburg, Germany and Houston, Texas, US
An Interview with Mr. Durgesh Sanjivrao Chandavarkar
Pat Walsh Texas Refinery Corp. One Refinery Place Ft. Worth, TX 76101
Mike Washington The Lubrizol Corporation 29400 Lakeland Blvd. Mail Drop 051E Wickliffe, OH 44092
Industry Calendar of Events
Ruiming “Ray” Zhang R.T. Vanderbilt Company, Inc. 30 Winfield St. Norwalk, CT 06855
Fundamental Study of the Initial Agglomeration of Lithium Soap Thickener in Lubricating Oil
Paul Shiller, Nikhil Prasad, and Gary Doll The University of Akron
CO-CHAIRS ACADEMIC & RESEARCH GRANTS: Chad Chichester Molykote 2200 W. Salzburg Rd., C40C00 Midland, MI 48686
EDUCATION: David Turner CITGO 1293 Eldridge Parkway Houston, TX 77077
EDITORIAL REVIEW COMMITTEE CHAIR: Joe Kaperick Afton Chemical Corporation 500 Spring St. Richmond, VA 23218-2158
TECHNICAL EDITOR: Mary Moon, PhD, MBA Presque Isle Innovations LLC 47 Rickert Drive Yardley, PA 19067
ON THE COVER Summertime Published bi-monthly by NLGI. (ISSN 0027-6782) CRYSTAL O’HALLORAN, Editor NLGI International Headquarters 118 N Conistor Street, Suite B-281, Liberty, MO 64068 Phone (816) 524-2500, FAX: (816) 524-2504 Web site: http://www.nlgi.org - E-mail: firstname.lastname@example.org The NLGI Spokesman is a complimentary publication. The current issue can be found on the NLGI website. The NLGI Spokesman is indexed by INIST for the PASCAL database, plus by Engineering Index and Chemical Abstracts Service. Microfilm copies are available through University Microfilms, Ann Arbor, MI. The NLGI assumes no responsibility for the statements and opinions advanced by contributors to its publications. Views expressed in the editorials are those of the editors and do not necessarily represent the official position of NLGI. Copyright 2018, NLGI. Send e-mail corrections to email@example.com.
PRESIDENT'S PODIUM Joe Kaperick Afton Chemical NLGI President 2018-2020
NLGI Annual Meeting – What Happens in Vegas? Perhaps some of what happens in Vegas should stay there, but if you’re attending the NLGI’s 86th Annual Meeting in the Red Rock Canyon area of Las Vegas, NV on June 8-11, 2019, there are quite a few things that you should take home with you. • The information and insight presented by Piet Lugt, Senior Scientist at SKF Research and Technology Development should be invaluable as you work to provide better solutions to you customers. As NLGI’s featured Industry Speaker, Piet will focus on the Basics of Bearing Lubrication including calculation models, new test methods, field data and more. Piet will lead off the Technical slate of talks on Monday morning. • The initials CLGS would be a great addition to your business card and something you can take anywhere with you to add value to your credentials as a Certified Lubricating Grease Specialist. The exam will be offered Tuesday afternoon during the conference. • The 29 Technical Presentations offered during the conference should provide you with a wealth of details to take with you. Papers will cover the gamut of grease topics ranging from production to testing to applications throughout the day on Monday and Tuesday. • Connections made from meeting Students and Professors from Academic Institutions and updates on the research that they have started using NLGI Research Grants will be critical for current or future understanding of the technical field. You may also return with solutions to recruitment needs as the next generation of grease researchers are introduced. Look for Lunch’n’Learn updates on Monday and Tuesday. • Updates on the newest developments and progress made by the various Working Groups will be available for you on Sunday afternoon. As well as the opportunity to continue to actively take part in any one of these groups outside of the Annual Meeting. This allows you to have input into the development of the next NLGI Grease Specifications, new test methods in Particle Evaluation or Bio-Based Greases or the latest in Food Grade Greases. • You can also take home an advanced understanding of the finer points of grease by taking advantage of the Basic and Advanced Grease Education Courses offered on Monday and Tuesday. • Finally, take home new contacts with suppliers, customers and technical experts in the grease community by taking advantage of all of the networking opportunities throughout the conference including Receptions (Saturday and Sunday evenings), Opening Ceremony (Sunday evening), Company Exhibits in Meeting Central (Sunday through Tuesday) and the Closing Night Celebration/Dinner on Tuesday evening. So if you’re coming to the Annual Meeting make sure that you take full advantage of all of the opportunities available to you and don’t go home empty-handed! For all other information (hotel, schedule, table top, education courses, and sponsorships), visit the NLGI website: 2019 Annual Meeting Info
We look forward to seeing you June 8-11 in Las Vegas! -3VOLUME 83, NUMBER 1
Exploratory Studies on Borate Esters as Dropping Point Enhancers Vennampalli M., Pokhriyal N.K., Bansal V. R., Saxena D. and Ramakumar S.S.V Indian Oil Corporation Limited, R&D Centre, Sector 13, Faridabad, India Abstract Borate esters are known for enhancing the dropping point of lubricating greases containing lithium 12-hydroxystearic acid-based soap. Several vendors are supplying packages of dropping point enhancers with different compositions and formulations of borate esters. Even though this technology is not very new, the basis of selecting a suitable dropping point enhancer is not clear. There are only a few studies showing their effectiveness as complexing agents added at the end of the manufacturing process. However, more studies on storage stability and effects on other properties in comparison to complex greases with boric acid are required. The performance of these additives is thickener-dependent, and the borate may liberate alcohol which either remains in the grease or evaporates out. In this paper, the authors discuss the evaluation of different dropping point enhancer borate ester packages and the development of a lab-prepared borate ester to enhance the dropping point of lithium soap greases thickened with lithium 12-hydroxystearate with respect to process, physical and chemical properties. The dropping point of lithium 12-hydroxystearic acid-based grease was 202°C; the lab-prepared borate ester enhanced its dropping point to 269°C, and to 276°C in the presence of zinc dialkyldithiophosphate. Key Words: Lubricating Grease, Lithium Soap, Borate Ester, Dropping Point Introduction Simple lithium soap greases thickened with lithium 12-hydroxystearate (Li 12-HSA) and having dropping points 175-210°C are widely used for moderate-temperature applications. The production and use of lithium complex soap greases is steadily increasing and was reported to have reached 20.04% of the global grease volume in the 2016 NLGI grease production survey. For high-temperature applications, complex soap greases are formulated with conventional complexing agents, usually a dicarboxylic acid such as azelaic or sebacic acid, with the 12-hydroxystearic acid. But, the complexing acids are comparatively expensive and/or require multi-step and high-temperature manufacturing processes to get grease with an effective dropping point. These complex greases generally need high thickener content and correspondingly more lithium hydroxide monohydrate to neutralize dibasic acids, which will increase the cost of the finished grease. Recent multifold rise in the lithium price is driving grease manufactures to look for cost cutting in all the aspects of grease manufacturing while maintaining the properties. Lower cost complexing agents such as acetic acid or benzoic acid do not give good high dropping point greases. Boric acid is a lower cost and good complexing acid which has been shown to result in Li 12-HSA complex greases with high dropping points. The borate complexing can be done in two ways: 1. By addition of boric acid or lithium borate at initial stages, which requires high-temperature processing up to 220°C to result in a complex grease with high dropping point [5,6]; 2. By addition of an activated ester of boric acid at the finishing stage of manufacturing. In the recent past, several reports have been published on lithium complex grease with borate esters. Kaperick et al. focused on complex issues of dropping point enhancement. An interesting article by Fish discussed about “Lubricating Grease Thickeners: How to Navigate Your Way Through the Lithium Crisis” -4VOLUME 83, NUMBER 2
and about borate esters as complexing agents in lithium and calcium greases. Research articles by Deshmukh  and Lorimor  have discussed borate complexation in lithium greases. Information In this paper, the authors compare methods of carrying out borate complexation in Li 12-HSA grease with boric acid, lithium borate and borate esters. Physical and chemical characteristics of the resulting greases such as consistency, dropping point, mechanical stability, roll stability and copper corrosion are evaluated. Several vendors are supplying dropping point enhancer packages for greases with different compositions and formulations of borate esters. We have evaluated three commercial dropping point enhancer packages with respect to the effect of alcohol used to make the borate ester, their addition temperature and hightemperature properties of additized grease. In order to reduce cost and develop homegrown technology, the authors have synthesized a borate ester and evaluated it against commercial borate esters. In the present study, the authors have investigated ways of making borate complexes using different forms of boron in a Li 12-HSA grease by selecting boric acid, lithium borate and a borate ester (activated ester). The first lithium complex grease was prepared using 12-hydroxystearic acid, boric acid and glycerol as a stabilizing agent. The second lithium complex grease was prepared using 12-hydroxystearic acid and lithium borate. The third grease was directly complexed with lab-synthesized borate ester (LBE). Further, the authors have investigated different commercially available borate esters along with the LBE synthesized in their laboratory. In this work, the suitability of borate esters with and without zinc dialkyldithiophosphate (ZDDP) and the effect of the alcohol used for making borate esters was also studied. Three greases were made with three different commercial dropping point enhancer packages, and one was made with LBE. The Li 12-HSA grease without a borate ester was considered as the base grease. Materials The base oil used was ISO VG 150 grade mineral oil. An antioxidant was also added to the finished grease. Commercial borate ester packages available in the market were used as dropping point enhancers along with the LBE. Equipment Standard equipment conforming to ASTM test methods was used for evaluation of physical and chemical properties such as dropping point (D2265), penetration (D217), copper corrosion (D4048) and roll stability (D1831). A JEM 6610L-JEOL scanning electron microscope (JEOL, Ltd., Tokyo, Japan) was used to obtain SEM images. Procedure All greases were prepared by batch (4 kg) process in a pressure reactor. The processing temperature was increased by one degree per minute, and the final temperature for batches with 12-hydroxystearic acid, boric acid and lithium borate was 220Â°C while for simple Li 12-HSA grease it was 200Â°C. A small excess stoichiometric amount of lithium hydroxide monohydrate used to keep finished grease alkaline (0.05-0.2 wt%). Main Steps Lab-Synthesized Borate Ester (LBE) After screening several alcohols such as linear, branched, primary, secondary, aromatic alcohols, diols, etc. for synthesis of borate esters, a branched alcohol was selected. This LBE resulted in a moderate flash point and boiling point. This ester was characterized by 1H, 13C and 11B NMR, IR spectra and flame tests.
-5VOLUME 83, NUMBER 2
Grease Manufacturing Gr-1: Lithium complex grease was made by addition of boric acid and glycerol in the initial stage along with lithium hydroxide monohydrate and 12-hydroxystearic acid in a pressure reactor. Gr-2: Lithium complex grease was made by addition of lithium borate in the initial stage along with lithium hydroxide monohydrate and 12-hydroxystearic acid in a pressure reactor. Gr-3: Lithium grease was made by reacting lithium hydroxide monohydrate and 12-hydroxystearic acid in a pressure reactor. This grease was considered as base grease and used as a reference for evaluation of borate esters. Gr-4: Base grease (Gr-3) was additized with LBE at 2 wt% at 90Â°C. Gr-5 to Gr-7: Base grease (Gr-3) was additized with three different commercial borate ester packages at 2 wt% at 90Â°C. Gr-8: Base grease (Gr-3) was additized with a 2 wt% mixture having 99.4 wt% LBE and 0.6 wt% ZDDP. The dropping point and other physical and chemical properties of the above greases were evaluated. Data, Observations and Results Physicochemical properties of greases prepared using different types of boron complexing agents are given in Table 1.
-6VOLUME 83, NUMBER 2
Table 1. Physical and chemical evaluation of greases with boric acid and borate(s) as complexing agents From Table 1, it is confirmed that all three lithium complex greases with boron had higher dropping points (258-269Â°C) than the base grease (202Â°C) But, making lithium complex greases with boric acid and lithium borate needed higher thickener content to result in NLGI grade 2 grease and the manufacturing process required more time and higher temperatures than simple lithium soap grease. Another disadvantage was that when boric acid was used in the initial stage, it consumed a corresponding amount of lithium hydroxide for neutralization, resulting in an overall increase in the cost of the product. However, by using borate ester as an additive, greases can be customized with higher dropping points. Additization of the base grease with borate ester was a faster approach to manufacture lithium complex greases. Production of lithium complex grease using a borate ester resulted in reduction of processing time and lower quantities of lithium hydroxide.
-7VOLUME 83, NUMBER 2
Table 2. Physical and chemical evaluation of greases with borate esters as complexing agent
-8VOLUME 83, NUMBER 2
Greases additized with borate esters were found to show either similar or superior physical and chemical properties to the base grease. Since this study was planned to evaluate effects of borate complexation only on the high-temperature properties of greases, extreme pressure additives were not added and a tribological evaluation was not done. Physicochemical properties of greases formulated with commercially available borate esters as dropping point enhancers and the LBE are given in Table 2.
Alcohol properties used in synthesizing a borate ester also play an important role in some aspects such as dropping point enhancement, flash point of the ester and evaporation loss of the grease. If a volatile alcohol is used, it can cause safety issues in the manufacturing process, even if the addition of the borate
Lithium complex greases can be conveniently and economically formulated with borate esters. The authors have looked into commercially available borate ester dropping point enhancer packages, which were found to be mixtures of borate esters and ZDDP. It was reported that ZDDP can also increase the dropping point to some extent in Li 12-HSA greases. The authors have evaluated three packages from different sources and compared them with a mix of LBE and ZDDP. All three commercially available dropping point enhancer packages were found to raise the dropping point of the base grease by 30-60째C at 2 wt% treat level. Greases Gr-5, Gr-6 and Gr-7 (with Packages 1, 2 and 3, respectively) resulted in dropping point enhancements to 253, 261 and 270째C, respectively. Grease Gr-8 formulated with a blend of 99.4 wt% LBE and 0.6 wt% ZDDP (equivalent to the ZDDP in commercial packages) at 2 wt% treat level gave the highest dropping point enhancement to 276째C (Table 2).
-9VOLUME 83, NUMBER 2
ester is done at the finishing stage (temperature around 8090째C). Branched alcohols are a better choice for making borate esters since they can stabilize the borate complex in grease through complex structure and have high flash and boiling points, thus making them safer to use.
During storage, stability of structure is essential to keep grease suitable for market applications. The authors have studied the properties of the greases that were stored for one year. As shown in Table 3, the borate ester-additized greases retained their structure and their high-temperature properties. No significant change in dropping point, mechanical stability and other properties was observed.
Table 3. Storage stability greases with borate ester as complexing agent after one year - 10 VOLUME 83, NUMBER 2
To understand the borate complexation in these greases and the mechanism involved in the enhancement of dropping points, an SEM was utilized to see any differences in the thickener fiber structures. From Figures 1 (a) and 1 (b), significant changes in fiber structure are obvious. According to Siegart and Henry , the borate ester forms a coordinated compound by sharing electrons between the boron atom of the borate ester and the hydroxyl group of the hydroxy fatty acid soap. The coordinated interactions between soap and complexing agent hold oil intact within the thickener structure at high temperatures, which leads to a high dropping point. Thus, it can be postulated that borate ester, being an activated ester, has lower activation energy to form a coordinated complex with the hydroxyl group of the hydroxy fatty acid soap and alcohol will be liberated from grease, if it is volatile. The entire process is catalyzed by a slight excess of lithium hydroxide. The cumulative/synergic effect of borate ester and ZDDP is very commonly used by grease formulators to enhance the dropping point.
Figure 1. SEM images of grease (a) without and (b) with borate complexation Conclusions Complexing of lithium soap with boric acid by conventional methods requires a high-temperature manufacturing process and additional amount of lithium hydroxide. Borate complexation in lithium 12-hydroxy stearate-thickened grease in the finishing stage with borate ester is a simpler, faster and more economical method of producing lithium complex greases. Using suitable alcohols having high flash points and boiling points to make borate esters will minimize safety issues when manufacturing complex greases. In a nutshell, it can be concluded that: • A borate ester was synthesized successfully from a branched alcohol and characterized in the authors’ laboratory. • The lab-synthesized borate ester at 2.0 wt% treat level worked as a dropping point enhancer in lithium 12-hydroxystearate grease. • Around 70°C increase in dropping point of lithium soap base grease was achieved with the lab-based ester and ZDDP. • Performance of the LBE was found comparable to that of three commercial dropping point enhancer packages that contained borate esters and ZDDP. • The properties of the LBE-additized grease did not change significantly when the grease was stored over a year. In the future, tribological evaluation of borate ester-additized greases, effects of other performanceimproving additives and effects on other thickener systems will be studied. - 11 VOLUME 83, NUMBER 2
Acknowledgements The authors are thankful to the management of Indian Oil Corporation Ltd. Research & Development Centre for granting permission to publish these data. References 1. Murray, J. L., “Lithium Complex Greases in NLGI Production Survey”, NLGI Spokesman, 45, 9, p. 309, Dec 1981 2. NLGI Grease Production Survey Report, 2016 3. “An Evaluation of sebacic acid and azelaic acid as thickeners in Lithium Complex Greases” by Tuszynski, W. and Bessette, P. A., NLGI Spokesman, 72, 4, pp. 30-37, July 2008 4. Exxon Research and Engineering Co., US Patent 5,391,309, Jan 24, 1994. 5. Mobil Oil Corporation, US Patent 3,842,008, May 18, 1973 6. Exxon Research And Engineering Co, US Patent 4,376,060, Mar 8, 1983 7. Kaperick, J. P., Aguilar, G., Garelick, K., Miller, A., Lennon, M. , Edwards, M., “Complex Issue of Dropping Point Enhancement in Grease”, NLGI Spokesman, 81, 6, pp. 36-45, Nov/Dec 2017 8. Fish, G. “Lubricating Grease Thickeners: How to Navigate Your Way Through the Lithium Crisis”, NLGI Spokesman, 82, 2, pp. 50-60, Mar/April 2018 (PAPER # 1713, Presented By Gareth Fish at NLGI 84th Annual Meeting, Olympic Valley, CA, June 10-13, 2017) 9. Deshmukh, V., Rajput, B.K. “Evaluation of Boron Esters in Lithium Complex Grease Prepared with Hydrogenated Castor Oil”, Preprint, Presented at the 82nd Annual NLGI Meeting, Coeur d’Alene, ID, June 6-9, 2015 10. Lorimor, J. “An Investigation into use of Boron Esters to improve High-Temperature capability of Lithium 12-Hydroxystearate Soap Thickened Grease”’ Presented at the 76th Annual NLGI Meeting, Tucson, Arizona, June 13-16, 2009 11. Yao, J., Zhao, J., Xi, Y. “The Antiwear Synergism between a Borate Ester and a Dialkyl Dithiocarbamate in Lubricating Oil and Grease”, Preprint, presented at the 72nd Annual NLGI Meeting, San Antonio, TX, Oct 30-Nov 1, 2005 12. Siegart, W. R. and Henry, C. J., US Patent 3,125,526, Mar 16, 1964
- 12 VOLUME 83, NUMBER 2
NLGI Hands-On Education Course SEPTEMBER 17-19, 2019
Koehler Instrument Company, Inc. | Holtsville, New York The class is taught in a participatory atmosphere, comprised of a Lecture section and a hands-on Laboratory Practical section where participants perform the prescribed test methods using the required instrumentation. Each participant will receive a course workbook upon arrival. Each day following the morning lecture section, participants will perform a selection of test methods discussed during the day using the required instrumentation. This hands-on approach will reinforce the topics and subject matter discussed during the lecture session to enhance learning and retaining knowledge.
• • • •
Scientists Plant Supervisors Laboratory Personnel Engineers
• • • •
Senior Technical Staff Maintenance Supervisors QC Staff Senior Plant Operators
$699 for NLGI members $799 for non-members
*Additional $100 may be applied toward membership dues if joining before 12/15/19.
Registration fee includes: • Course Workbook • Roundtrip transportation provided by the Courtyard by Marriott • Lunch & Reception
QUESTIONS? Contact NLGI HQ at 816-524-2500 or firstname.lastname@example.org
View SCHEDULE, HOTEL INFO AND REGISTRATION DETAILS online:
This course provides an excellent overview of the types of greases, thickeners, base oils and additives. The methods of manufacturing, testing methodology and their use in bearings and in industrial and automotive applications are also covered.
TOPICS: • • • • • •
Course Overview & Introduction to Greases Application Problem Solving Grease Manufacturing Overview Grease Testing Automotive Applications Industrial Applications
• • • •
Grease Selection and Recommendations Special Tests Applications: Grease Tribology Grease Composition - Base Oil Basics - Thickener Basics - Additives
A Novel Testing Approach to Validating Automotive Lubricant Performance in Fretting Conditions Dr. Jason T. Galary*
The reliability of components such as actuators, bearings, and electrical terminals in automotive applications is a critical factor related to warranty requirements and customer safety. Despite its importance, it can be very difficult and expensive to test component reliability. Historically, it has also been very difficult to produce repeatable data with bench testing, even with large sample sets, to provide useful results. This has driven the use of computer simulation modeling, which reduces testing time and cost with a much smaller computational impact, although component level or full application testing is still required by OEMâ€™s and Tier 1 suppliers . This paper presents a new benchtop apparatus, the multi-terminal fretter, to test and validate components like actuators and electrical terminals for their ability to protect against fretting conditions. This new methodology allows for various frequency and amplitude conditions to be tested to generate life probability curves and understand the improvements made by lubrication. In the present study, the multiterminal tester was applied to electrical terminals. It provided meaningful data and demonstrated its value for testing applications subjected to fretting conditions and showing how various lubricants help improve their reliability and extend their lives. KEY WORDS: Fretting, Electrical Contact, Connector Lubricant, Grease, Corrosion *Nye Lubricants, Inc., Fairhaven, MA Introduction and Background There has been a sharp increase in the volume of electrical and electronic components used in commercial, industrial, consumer, and military applications over the last decade. The life of these components is directly related to the reliability of electrical contacts. Along with reliability, safety is also of the highest concern for automotive applications, especially with the rise of hybrid and battery electric vehicles (BEV). Together, reliability and safety directly impact the perceived quality of automobiles, which tie to their quality and warranty aspects. With the global trend moving towards adding additional electronic controls to automotive applications, or complete conversion as is the case with electrical and hybrid vehicles (EHV), there can be more than 400 connectors with over 3,000 individual electrical terminals in an automobile . At the heart of these applications are the electrical terminals and contacts, which are subjected to oxidation, humidity, vibration, and fretting. The phenomenon of fretting wear refers to small amplitude, relatively high frequency oscillatory slip motion between two bodies in contact. In automotive applications, vibrations or thermal cycling can cause fretting due to very small oscillations that range from fractions of a micrometer up to about 100 Âľm. For electrical terminals and other components, this amount of relative movement between mated components leads to several types of surface damage that result in fretting corrosion and wear. In fretting wear, the top layer of material is removed due to pure mechanical wear.
- 14 VOLUME 83, NUMBER 2
Fretting corrosion occurs when there is a passive film on a surface in the contact. This passive film is a very thin layer of oxidized corrosion byproducts that forms on the nascent metal and leads to increased contact resistance and loss of continuity. Fretting is typically caused by vibrations in a system or by temperature cycles and variations that cause expansion and contraction. As fretting occurs in a system, pressure can force a terminal through the contact surface to cause wear. As time goes on, the wear oxidizes and hardens the surface. Because of the small amplitude vibrations, particles of oxidized wear material have difficulty escaping from the contact zone where they continue to cause additional wear and oxides. As this wear happens and oxides form, the contact resistance in the terminal increases until continuity is lost. Figure 1 shows a kinetic model of fretting wear and corrosion.
Figure 1: Kinetic Model of Fretting Wear and Oxidation In a lubricated contact, the lubricant provides a film that separates the moving surfaces and carries the wear particles out of the contact to help prevent additional wear and oxidation. The general research into fretting wear that has been performed and published over the years heavily focused on bearings and power train applications . The ASTM D4170 method “Standard Test Method for Fretting Wear Protection by Lubricating Greases” was the main method of evaluation used for much of that research . D4170 evaluates the ability of lubricating greases to protect an oscillating bearing from fretting wear and differentiates the performance of formulated lubricants. Additionally, work was done around the proper formulation of a lubricating grease for performance in D4170    and tied to the development of high-performance wheel bearing greases and their specifications  . It is estimated that over 60% of the electric problems in cars are caused directly by fretting, and this problem could increase in the future with the expanded use of EHV’s  . Because of this trend, fretting wear is one of the major mechanical forms of deterioration and failure of electrical terminals and contacts. There are many well-known applications where connectors are mounted to an engine, exhaust system, etc., and vibrations, as well as extreme temperature cycles, occur when the engine runs. In underhood applications, exhaust gases can accelerate fretting corrosion. All of these factors combine to make a very complex problem that leads to lowered reliability and possible warranty issues. - 15 VOLUME 83, NUMBER 2
To improve the durability and reliability of automotive components under fretting conditions, lubricants are known to help extend the operational life of the contacts. This is accomplished in several ways. First, the lubricant helps reduce friction by forming a thin film between mating surfaces, which leads to an ease of sliding surfaces. Second, lubricants help seal porous coatings in electrical terminals where substrates such as copper can ‘bloom up’ through porous metals such as gold and cause advanced fretting corrosion. Finally, lubricants help protect against oxidation corrosion by insulating the lubricated contacts from the environment, which prevents oxide formation and more aggressive wear. The study of fretting behavior of electrical terminals has been heavily researched    . The fretting wear of various automotive components, including electrical terminals and connectors, has been studied at the research level and by commercial manufacturers. Their research showed that currently, fretting testing is being done with computer simulations, experimental simulations using bench tests and generic specimens (crossed cylinders, cylinder on plates, etc.)  , and electrical terminals subjected one at a time to mechanical vibrations or heat cycling. The experimental simulation approach using generic test specimens has two main weaknesses. First, this approach uses a very small set of specimens, which makes it difficult to show statistical significance. Second, the geometry of the specimens can produce results that do not correlate well to commercial mechanisms. This has led to the development of the multi-terminal fretter (MTF) , which can evaluate as many as ten electrically isolated terminals at the same time for statistical significance. The design for the MTF is shown in Figure 2. Experiments Testing Methodology The MTF is made up of two electrically isolated testing blocks, one stationary and one oscillating. Various components are fixtured to these blocks for testing. A power source is applied, and a four-wire resistance measurement taken across the testing specimen. Once a test specimen is fixtured on the testing blocks, a linear actuator with absolute encoder is used to oscillate the testing stage and create the fretting wear testing profile. The frequency of oscillations is controlled by a voice coil actuator that allows for accurate motion control down to 1 µm over the fretting range. This operates on the principle of a magnetic field around a coil winding to generate a force (Lorentz Force) when current is applied to the coil. When a test is fixtured and set up, great care is taken for the alignment of the components, specifically electrical terminals, to prevent issues caused by misalignment. A typical test is performed by first measuring the static resistance of the fixtured sample, and then continuously reading the 4-wire resistance until the failure criterion is met or the preset number of test cycles is exceeded. As the MTF can run multiple samples at the same time, the test continues until all samples fail. Typically, a 100 to 500 mΩ change in contact resistance constitutes a failure. This has been accepted as a representative failure level by the automotive industry   .
- 16 VOLUME 83, NUMBER 1
Figure 2. Multiple-Terminal Fretter Apparatus Test Configurations In this study, electrical terminals were tested in three different styles with low and high frequency oscillations and unlubricated and lubricated contacts. All testing was performed in an environment of 23 +/- 2 C and 40 +/- 5% relative humidity. i. ii. iii.
2.8 mm beryllium copper electrical terminals Completed electrical connectors using 1.5 mm terminals and receptacles 1.5 mm electrical terminals used in the completed connector package
Figure 3. 2.8 mm Terminals
Figure 4. Completed Electrical Connectors
- 17 VOLUME 83, NUMBER 2
Figure 5: 1.5 mm Electrical Terminals Two different testing plans were used in this study. The first plan focused on testing bare 2.8 mm beryllium copper electrical terminals. The second plan used fully assembled electrical connector packages for automotive heat controller applications, as well as the individual terminals, to simulate a finished assembly and the straight subcomponent terminals. The conditions for these simulations were 10 Âľm amplitude oscillations at 10 Hz (low frequency test) as well as 10 Âľm amplitude oscillations at 100 Hz (high frequency test). Before testing, the electrical terminals were cleaned ultrasonically in mineral spirits followed by acetone. The testing apparatus was then assembled with 0.2 mg of lubricant added to the female terminal. For dispersion testing, the male terminal was dipped. Careful attention was paid to the alignment of the terminals, and then, the testing fixture was secured. Testing was run at an ambient temperature of 23 C and 40% relative humidity, with no external load apart from the spring in the electrical terminal design. The testing was then performed with 10 cycles of coupling/uncoupling of the terminal pair to precondition the materials. After the precondition step, the test was static for 1 min while the baseline resistance was measured. Resistance readings were taken every 1 s with up to 10 readings on each channel. Then, oscillations at the test frequency and amplitude were performed until the average resistance over a 30 s period increased by more than 500 mÎŠ, which indicated a loss of continuity and failure due to fretting corrosion. Materials Two materials were tested in this study: i. Polyurea thickened grease based on a PAO/alkylated naphthalene oil blend of 193 cSt at 40 C ii. A 20% dispersion of the above grease in isoparaffinic solvent. Analysis Software Minitab statistical software was used to calculate Weibull life probabilities from test data . In general, a large number of samples is required to accurately estimate Weibull parameters. In this study, each evaluation had between 10 and 20 replicates to provide a large enough sample set of failure data to estimate the Weibull life probability. The mean, median, and 90% confidence intervals were calculated for all of the Weibull parameters and converted to life percentiles. The F90, F50, and F10 values were calculated; they represented the number of cycles until 90, 50, and 10% of the component population failed. The F50 value was used to represent lubricant life .
- 18 VOLUME 83, NUMBER 2
Results and Discussion 2.8 mm Fretting Tests The results in Table 1 and Figures 6 and 7 are for the 2.8 mm terminals in the high and low frequency tests for both dry and lubricated conditions. These Weibull life probability plots illustrate that the grease significantly improved the durability of these electrical terminals versus the unlubricated contacts for both high and low frequency oscillations.
Figure 6. 2.8 mm High Frequency Fretting Results
Figure 7. 2.8 mm Low Frequency Fretting Results
Table 1. Weibull Life Probabilities for 2.8 mm Terminals - 19 VOLUME 83, NUMBER 2
Figures 6 and 7 also show the results for the 2.8 mm terminals lubricated with a 20% dispersion of the grease in isoparaffinic solvent. While the 20% dispersion of grease in solvent did provide some improvement in life of the electrical terminals, it was significantly less improvement than the effect of the grease at both high and low frequencies. The reason for this difference in performance was based on the film thickness and amount of lubricant available to replenish the contact and protect the surface. When the lubricant was only 20% grease dispersed in a solvent, its oils and additives were depleted much sooner than in the case of the undiluted grease. Thus, the dispersion of grease in solvent was less successful than the grease at sealing the surface of the contact. Connector Package Fretting tests The results in Table 2 and Figures 8 and 9 are for the fully assembled connector package terminals tested at high and low frequencies for both dry and lubricated conditions. These Weibull probability plots illustrate that the grease and the 20% dispersion of grease provided a significant increase in the durability of the electrical terminals over the performance of unlubricated terminals under both high and low frequency conditions.
Figure 8. Assembled Connector High Frequency Fretting Results
Figure 9. Assembled Connector Low Frequency Fretting Results - 20 VOLUME 83, NUMBER 2
Table 2. Weibull Life Probabilities for Assembled Connectors 1.5 mm Terminals from Connector Package Fretting tests The results in Table 3 and Figures 10 and 11 are for the terminals tested by themselves (not in connector packages). These Weibull probability plots illustrate that the grease and the 20% dispersion of grease provided a significant increase in the durability of the electrical terminals over the performance of unlubricated terminals under both high and low frequency conditions.
Figure 10. Assembled Connector High Frequency Fretting Results
Figure 11. Assembled Connector Low Frequency Fretting Results - 21 VOLUME 83, NUMBER 2
Table 3. Life Probabilities for 1.5 mm Connector Pins Discussion The results of these three fretting experiments indicated that lubrication improved the reliability and durability of the electrical contacts. This improvement in life expectancy of the lubricated contacts can be attributed to several factors: i. Ability of the lubricant or additive package to prevent oxidation corrosion. ii. Reduction of wear in the contact Through passivation of surface oxides and removal of fresh nascent metal wear particles from contacts, the severity of abrasive wear was greatly reduced, as seen in Figures 12-15. The contacts tested with grease had the longest life probability and the least amount of wear. The greased samples performed the best in this study, as these greases contained additives for passivation of metals and protection of the contact surfaces. In the case of the dispersions of 20% grease in solvent, the life and wear of contacts were improved over dry (no lubricant) samples, but contacts were still less durable than those lubricated with grease. As the dispersion only contained 20% of the lubricating grease, its additive package was depleted sooner, and there was no mobility of remaining lubricant as it was simply a thin film coating.
Figure 12. Wear of 2.8 mm Terminals (Low Frequency)
- 22 VOLUME 83, NUMBER 2
Figure 13. Wear of 1.5 mm Terminals (Low Frequency) The wear patterns on the 2.8 mm terminals were very consistent, while the 1.5 mm pins showed a random placement of the wear scars (Figure 13). All of the wear patterns for these 2.8 mm pins always had a central circular wear track from the contact in the female receptacle along with a smaller track on either side. However, the 1.5 mm pin terminals all had random placement of this wear scar with combinations of centrally located wear scars along with scars on either side of the contact This random wear pattern occurred in the pre-assembled connectors and the individual 1.5 mm terminals. After investigating this random wear pattern, it was found that the male and female receptacles for this connector package were not matched properly. Because of this mismatch, there was additional play in the package, which led to contact at random spots on the pin when mated. This illustrates a potentially serious issue, as the contract stress distributions differ on the center of the terminal versus the edge, which could lead to a larger amount of variation in the life of the electrical terminal. This observation emphasizes the importance of making sure that the components are properly matched. To investigate this further, surface topography using a profilometer was performed on several wear scars as seen in Figures 16 and 17.
- 23 VOLUME 83, NUMBER 2
Figure 14. Wear of 2.8 mm Terminals (High Frequency)
Figure 15. Wear of 1.5 mm Terminals (High Frequency) - 24 VOLUME 83, NUMBER 2
The wear surface profiles shown in Figures 16 and 17 were acquired using a Taylor Hobson Talymap Profilometer. The color corresponds to depth in each surface profile. Profiles were taken from several 1.5 mm terminals used in this testing to further investigate the concerns about contact stress distribution related to the random placement of wear scars. On terminals that had wear scars along their edge, the average wear volume lost was 70,500 Âľm3, while the centered scars were under 9,000 Âľm3. This dramatic difference in wear volume was attributed to a smaller area of contact with the mating terminal, which resulted in higher contact stress and larger wear volume.
Figure 16. Surface Wear Topography (Edge Scars)
Figure 17. Surface Wear Topography (Center Scars)
Table 4. Life Probabilities Comparison for Connectors and Pins - 25 VOLUME 83, NUMBER 2
Comparing results from all three experiments shows that these results all follow the same trend for performance. The lifetimes for completed connectors lubricated with grease were much greater than either of the straight terminal tests. Looking at the assembled connectors after these tests, two discoveries were made. First, there was a significant degree of freedom in the overall movement of components. This allowed for the energy put into the connector through the fretting motion to be absorbed or redirected. Because of this reduction in the relative friction, lifetimes of the assembled connectors are expected to be significantly greater than the pins and sockets by themselves. (This initially drove the third experiment.) Second, the manufacturer of this automotive component used non-matching pins/sockets. This discovery clearly illustrates the need to exercise great caution when selecting non-matching components. In this case, the contact stress in the terminals was outside the desired range, which led to increased wear rates. These fitment issues and contact stress differences can also lead to uneven wear of contacts, which by itself can lead to discontinuity (failure) of contact resistance and application failure. Conclusions This study used a variable frequency multi-terminal fretting (MTF) tester to evaluate component level electrical terminals and completed connector assemblies, and the effects of dielectric lubricants on reliability and durability of these components. The use of a dielectric lubricant (grease or dispersion of grease in solvent) greatly improved the durability of the electrical terminals and connectors. For the 2.8 mm terminals, the durability was increased by ~24 times in the high frequency testing (100 Hz) and 7 times in the lower frequency tests (10 Hz). This life improvement was directly tied to the reduction of oxide formation in the electrical contact, which drives the amount of abrasive particles produced. While the overall life of the electrical contact was better at low frequencies, the durability improvement over dry unlubricated contacts was greater with the high frequency than low frequency testing. This difference was related to sliding speed in the contact and how the lubricant film formed. As the speed increased in a contact, a strong EHD film was created, separating the surfaces and pushing the particles out of the contact. The assembled connectors, as well as the separate 1.5 mm pins and sockets, showed similar results but with much greater increase in durability compared to dry terminals. In these tests, the improvement from the pin/socket tests to the connector assemblies ranged from 2 to 11 times the durability in the life of the test. The improvements seen in the connector assembly testing were due in part to the fitting and amount of free body motion allowed in the connector, which helped to redistribute the force, reduce fretting, and allow for a longer test life. While this may be the case with all connector assemblies, this differential between the electrical terminals and assembled connectors is believed to be on the lower side of the range. From the results of this study, there was a significant improvement in durability and reliability of electrical terminals when a connector lubricant was used. Using the MTF test rig, similar performance results were seen when testing terminals, fully assembled connector housings, and the electrical terminals from those connectors. This is a critical point, as it illustrates that when using the MTF, an accurate experimental simulation of applications can be made using only the electrical terminals, which will save time, costs, and test complexity. It is also important to note the following findings from this study: i. All connector lubricants are not the same. An oil or dispersion of grease will not protect the electrical contact as well as a properly formulated dielectric grease. - 26 VOLUME 83, NUMBER 2
ii. An increase in frequency can reduce the time until the onset of fretting corrosion and reduce the durability of the contact. Acknowledgements I would like to thank the ADVT team at Nye Lubricants, specifically Gus Flaherty, Richard Bellizzi, and Mason Wood, for performing the testing and fabricating testing fixtures. References  Bolger, G. “The selection of automotive connectors”, Senior Thesis, Coventry University., U.K., 1997.  Law, D. A. and Rowe, C. N., “Fretting Wear with Powertrain Lubricants,” Lubrication Engineering, 43 (8): 616-622 (1986).  Verdura, T. M., “Development of a Standard Test to Evaluate Fretting Protection Quality of Lubricating Grease,” The NLGI Spokesman, 47: 157–67, (1983).  Schlobohm, R. T., “Formulating Greases to Minimize Fretting Corrosion,” The NLGI Spokesman, 45: 334-338, (1982).  Wunsch, F. G., “Relationship between the Chemical Structure of a Lubricant and Fretting Corrosion,” The NLGI Spokesman, 52:. 424-31, (1988).  Kaperick, J. P., “Fretting Wear – Something to Worry About?,” The NLGI Spokesman, 72 (4):. 19-29, (2008).  Kato, M. and Sato, T. “The Development of Low Friction and Anti-Fretting Corrosion Greases for CVJ and Wheel Bearing Applications,” SAE Technical Paper Series 871985 (1987)  Mishima, M., Kinoshita, H., and Sekiya, M. “Prevention of Fretting Corrosion to Wheel Bearings by Urea Grease,” The NLGI Spokesman, 53: 496-504, (1990).  Swingler, J. and McBride, J. W. (1998) The synergistic relationship of stresses in the automotive connector. Proceedings of the
19th International Conference on Electric Contact Phenomena. 01 Jan 1998. pp. 141-145 .  Swingler, J., McBride, J. W., and Maul, C. “Degradation of road tested automotive connectors.” IEEE Transactions on Components and Packaging Technologies, 23 (1): 157-164, (2000).  Hannel, S., et al. “The fretting sliding transition as a criterion for electrical contact performance.” Wear 249.9: 761-770, (2001) .  Achanta, S., et al. “Friction mechanisms at the micro-scale.” Tribology International 42.11-12: 1792-1799, (2009) .  Saka, N., Liou, M. J., and Suh, N. P. “The role of tribology in electrical contact phenomena.” Wear 100.1-3: 77-105 (1984).  Chowdhury, M. A. and Helali, M. M. “The effect of frequency of vibration and humidity on the wear rate.” Wear 262.1-2: 198-203, (2007).  Liskiewicz, T., Neville, A., and Achanta, S. “Impact of corrosion on fretting damage of electrical contacts.” Electrical contacts-2006, Proceedings of the Fifty-Second IEEE Holm Conference on. IEEE, (2006).  Achanta, S. and D. Drees. “Effect of lubrication on fretting wear and durability of gold coated electrical contacts under high frequency vibrations.” TribologyMaterials, Surfaces & Interfaces 2.1: 57-63, (2008).  Galary, J. “Investigation of Fretting Wear and Durability of Electrical Terminals when exposed to Variable Frequency Vibration”. JAST Transactions of the World Tribology Conference, (2015).  SAE/USCAR. “Performance Specification for Automotive Electrical Connector Systems” SAE/ USCAR-2, (2013).  Weibull, W. “A statistical distribution function of wide applicability.” Journal of Applied Mechanics, 18.3 : 293-297, (1951).
- 27 VOLUME 83, NUMBER 2
The Cost of Compromise: Wind Turbine Main Shaft Grease Lubrication Engineering Study Edward Worthington and Dwaine Morris Shell Product Technology Hamburg, Germany and Houston, Texas, US
Abstract Wind turbine main shaft and blade bearings have divergent lubrication requirements due to some specific application conditions and performance implications. Main shaft bearings are heavily loaded components subjected to slow rotational speeds, shock loads and variable ambient temperatures. While blade bearings are also subjected to similar conditions relative to load and temperature, they are further exposed to limited angle of rotation and are prone to fretting wear due to high frequency vibrations. To satisfy lubricating requirements, most main shaft greases tend to contain higher viscosity base oils, whereas blade bearing greases have trended toward lighter viscosity base fluids. However, there have been, and continue to be, attempts by original equipment manufacturers and turbine owners to utilize the same lubricating grease for these divergent applications. Wind turbine original equipment manufacturers are increasing base oil viscosity for blade bearing greases while simultaneously decreasing the base oil viscosities of main shaft greases. Their intents are to gain mobility and reduce low-temperature torque in the main shaft grease, while increasing the shock load resistance of the blade bearing grease and maintaining the fretting wear protection. For the OEMs and maintenance service providers, this consolidation reduces complexity. However, this consolidation compromises optimal performance in both applications. This paper examines a case study of a specific attempt where consolidating greases for main shaft and blade bearings led to excessive wear and risk of catastrophic wind turbine failure. The analytical tools and engineering calculations used in a root cause analysis in this case study can also be applied to predict the suitability of greases for main shaft bearings and other applications. Presented at the NLGI 85th Annual Meeting Coeur d’Alene, ID June 9 - 12, 2018 Background- Renewables on the Rise Wind energy is growing in significance in the US energy production market. According to the American Wind Energy Association (AWEA): • In 2012 wind energy became the number one source of new US electricity generating capacity, supplying 42% of the newly installed capacity.  • The turbines themselves are producing nearly 20 times more power per turbine than those installed in 1990.  • Together, renewables accounted for ~67% of newly installed power generation capacity in the US in 2015.  • In 2016, electricity generated from wind energy avoided 159 million metric tons of carbon dioxide emissions. This is the equivalent of reducing power sector CO2 emissions by 9% and avoiding the consumption of 87 billion gallons of water. 
- 28 VOLUME 83, NUMBER 2
Figure 1 US Energy consumption sources- 2017 and Renewable detail According to updated information from these same sources, wind power (Wind) now contributes over 6% of the US power generation capacity. In addition, for the most recent 5-year period (2013-2017) Wind accounts for 25% of the annual newly installed power capacity additions. - 29 VOLUME 83, NUMBER 2
As Wind becomes more prominent in newly installed capacity of the North American energy production matrix, its reliability becomes more critical as other portions of the energy portfolio begin to decline. As coal has waned as an electrical generation fuel, the contribution of ‘other renewables’ (Figure 1) and natural gas are expanding to close the demand gap.  As Wind becomes more prominent in the newly installed capacity, the longevity and reliability of wind turbine assets must be ensured. Setting aside all other challenges to operational efficiency in the turbine, reliability and operational availability for the blade and main shaft bearings must be considered as critical path. These two distinct applications have some common lubrication needs, but the primary failure modes are significantly different enough to warrant the application of unique grease solutions per application. Wind original equipment manufacturers (OEMs) have been migrating to grease consolidation to simplify manufacturing and installation. In addition, this reduces complexity for them during the period in which they are responsible for the upkeep of the ‘new’ turbines. In general, consolidation of products may appear to be a valid or even a good option, but in the case of wind turbine bearings, careful consideration of operational conditions and examination of potential outcomes provide more than enough reasons to pause and reconsider that approach. The following case study is an example illustrating that collective lubrication shared experience and engineering knowledge are more than adequate to provide a warning of potential negative outcomes from selection of an inappropriate lubricant. In this case study, the calculations predicted bearing distress in the applications. The long-term, real-world outcome verified these calculations. This case in particular should serve as a warning to OEMs and operators alike to exercise caution in the selection of lubricating greases for the main shaft grease. Due to confidentiality concerns for the OEM and the wind farm owner / operator, the identity of those parties is withheld from this paper. In addition, the geographic location of the facility is not disclosed for the same reasons. Historic ambient operating conditions are shared to illustrate the importance of selecting greases to prevent, or at a minimum, mitigate, damage before widespread failures become imminent. Introduction From location to location and fleet to fleet, main shaft bearings in wind turbines operate in a wide variety of environments. Ambient temperatures can range from -30 to 45 C . The rotational speeds hover in the range of 10-20 rpm during the generation cycle. The bearings experience shock loading, vibrations and heavy loads (C/P ratios from ~6 to 8). These conditions determine the requisite size and bearing design necessary to manage the shock and thrust loading. These same considerations should determine the correct grease selection. Due to confidentiality concerns of all parties, the exact bearing will not be discussed, but an analog double row spherical roller bearing is put forward for consideration with the following dimensions and load limits: Bearing ID 560 mm Bearing OD 820 mm Bearing Width 195 mm Dynamic Load Rating 5,600 kN Static Load Rating 10,200 kN 
- 30 VOLUME 83, NUMBER 2
Based on the above design and load specifications, available calculation tools indicated that the minimum viscosity required at the bearing operating temperature to maintain a Kappa value (viscosity ratio) >1.0 is 143 cSt. The Kappa value is defined as the ratio of the viscosity of the lubricating grease film divided by the minimum required viscosity at the bearing operational temperature. In this case study, the installed grease was an ISO 150, NLGI 1 lithium thickened grease fortified with extreme pressure additives. A cursory review would indicate that this grease would be acceptable for the normal operation of the main shaft bearing with a nominal Kappa value >1.0 at bearing temperatures up to ~42 C. After approximately 9 years of operation, main shaft bearing in-service grease samples contained high concentrations of wear metals. Consultation with lubricant suppliers verified that less than adequate fluid film was a major contributing factor in the excessive wear. The OEM and maintenance operations at the site instituted a mitigation plan that was intended to flush the wear debris and install a grease with higher viscosity base fluids. The maintenance program was not completely successful, and recent analysis of the in-service greases indicated an approximate 50/50 ratio of the fill grease and the mitigating grease (a synthetic ISO 460 polyurea thickened grease with extreme pressure additives). Wear metal analysis revealed copper in the range of 65,000 ppm and iron content in the range of 28,000 ppm. Wear metal species present in these quantities are indicative of significant cage and roller wear. These results are consistent with the expectations of bearing distress when the bearing is operating with Kappa values less than 1.0 or in lubrication starvation mode. The presence of high concentrations of wear metals was also catalyzing the oxidation of the in-service grease. Pressure differential calorimetry indicated no reserve oxidative life for the in-service grease. If allowed to continue in this condition, catastrophic failure was more than a possibility. A slow-motion disaster was a forgone conclusion, predicated on dubious assumptions and operational conditions that exceeded the performance limits of the installed grease in the main shaft bearing. Grease Selection Considerations The primary consideration for grease selection should be viscosity (and the corresponding lubricating film) at the bearing operating temperature. Care should always be taken to ensure that the chosen lubricating grease provides an adequate fluid film under extreme conditions as much as possible, but performance under the â€˜anticipated normalâ€™ conditions is essential. The primary failure modes, and the ability of the grease to mitigate those, are an important secondary concern. In the case of main shaft bearing greases, the major performance demands for the grease are load carrying capacity (EP and AW under loaded conditions), mechanical stability, oxidative resistance, mobility (in bearings and central lubrication systems), minimal starting / running torque and corrosion control. A secondary concern is fretting when the turbines are idle. In the case of a blade bearing greases, performance demands are nearly identical, except that fretting corrosion control is significantly more important due to the high frequency vibrations that can cause significant damage and failure in blade bearings. It is easy to understand the urge to consolidate lubricating grease products for these two applications, as these applications share so many common lubricating needs / challenges; however, consolidation can be dangerous. Within the wind industry, OEMs have developed test matrices that mimic the primary failure modes of bearings. These test regimes include some standard tests (Fafnir Fretting - ASTM D4170) and some wind specific tests, such as the impact fretting test and the Riffel test.    Each of the OEMs leans on their - 31 VOLUME 83, NUMBER 2
own versions of these tests to varying degrees or consults with bearing suppliers with regard to grease selection or qualification. According to Yano, there are relationships between fretting and load carrying capacity as measured by the specialized load carrying tests (Impact Fretting). 
Figure 2 Fretting wear in ASTM D4170 versus viscosity for selected grease products
Figure 2 illustrates relative wear performance in ASTM D4170 of selected greases from the Yano study. As viscosity increases, the ability of the product to protect the bearing from fretting wear decreases. In any population of greases, as in the Yano study, there is scatter regarding fretting wear. This scatter in test data is directly related to oil release properties of these products, and the oil release properties account for the variation in performance of products with nearly identical viscosity with regard to fretting. The importance of this general relationship between fretting wear and base oil viscosity hints at the OEM decision process when selecting the main shaft grease. It appears that the OEMs have been concerned about the secondary failure mode of fretting in the main shaft when they specified the main shaft bearing grease.
Figure 3 Impact fretting rating versus viscosity for selected products- lower ratings indicate better protection / performance in the test - 32 VOLUME 83, NUMBER 2
Yano observed that protection from impact fretting (related to load carrying) increased as oil viscosity increased (Figure 3), which is the inverse of the trend that protection from fretting wear decreased as oil viscosity increased (Figure 2). Figure 4 shows that there is an inverse relationship between impact rating (load carrying) and fretting wear for greases. To have the required load carrying capacity (related to the viscosity), grease formulators must trade off between these two performance characteristics. Thus, using the same grease in main shaft bearings (where load carrying is a priority) and blade bearings (where fretting resistance is a priority) comes with an inherent compromise.
Figure 4 The ASTM D4170 performance of selected greases plotted against their corresponding impact rating If the intent is to choose a single, consolidated grease product, a logical approach would be to identify a product that would meet the primary performance requirements related to viscosity and load carrying capacity, while maximizing fretting protection. By selecting a product that has oil release properties and bearing mobility that provide some level of fretting protection, it might be possible to find a consolidated grease solution. Figure 5 shows a plot of ASTM D4170 fretting wear on the primary axis and impact rating on the secondary axis versus base oil viscosity for a set of grease products. From this plot, it is possible to identify those products that are theoretically capable of achieving adequate performance in both screening tests. The logarithmic trend lines for the two sets of test data cross at approximately ISO 150. The region where the lines intersect indicates products with the potential for compromise with â€˜middle of the roadâ€™ performance in both measures. Recall that the calculated minimum required viscosity for the main shaft bearing is 143 cSt.
- 33 VOLUME 83, NUMBER 2
Figure 5 Fretting wear and Impact rating plot versus viscosity, looking for a compromise product. Red line indicates impact rating while the blue line indicates fretting wear The authors are not privy to the thought process specifically, but this seems to be a logical progression given the openly available performance information and literature on the subjects. However, the specific performance issue related to this installed fleet was due to the assumption of bearing operating temperature. If the assumptions were that the bearings would not exceed 40 C, then the location and historical ambient temperature data should have been checked and verified. During the analysis phase of the product selection process, it is important to establish the estimated bearing temperatures to project the efficacy of the chosen product for the fleet location. Once the authors were contacted to conduct the failure analysis and mitigation for the site, the first step was to determine the required viscosity for the operating bearings and then determine what the projected operational bearing temperatures would be under normal and extreme circumstances. Consider the following:
Figure 6 Installation average daily temperature from 2015-2017 - 34 VOLUME 83, NUMBER 1
Historical ambient temperature for the site from 2015-2017 in Figure 6 revealed that the average temperature did not exceed the limit of the chosen grease (42 C) to provide adequate fluid film for the bearing. However, the bearing temperatures would be elevated above the projected average for an extended amount of time based on loading and the fact that the high temperatures would considerably exceed the average. In fact, the analysis in Figure 7 confirmed this:
Figure 7 Moving average temperature, daily high temperature and the projected daily high bearing temperature The projected daily high bearing temperatures, based on ambient +20 C, would ensure that the bearing would be operating a significant portion of the time in a region of surface distress based on the installed greaseâ€™s published base oil viscosity and its projected response to temperature, Figure 8:
Figure 8 Projected viscosity of installed grease and an ISO 460 synthetic grease as bearing temperature rises
- 35 VOLUME 83, NUMBER 1
Based on loading, the calculated projected bearing temperatures corresponding to the temperature estimates plotted in Figure 7, with the average operating temperature of the bearing at 25 C ambient was 52 C, exceeded the limits of the installed grease to provide adequate film for the operation. The average daily high temperature over the three-year period from 2015 to 2017 was 24.4 C. This would invalidate the assumption that, the bearing operating temperature is less than 42 C, Figures 7 and 9. Feedback from the site confirmed that recorded bearing temperatures aligned with the projected and calculated values. The resultant viscosity of the installed grease ensured that the bearings were operating where their surfaces would be distressed on approximately 60% of the days (~220 days per year), and even at the lowest ambients, the bearing operational temperatures would be in excess of the performance limit of the installed grease ~50% of the time, Figure 9.
Figure 9 View of projected bearing temperature and the distress point of the installed grease The previous analysis is predicated on the steady state assumption, meaning that the turbine shaft is rotating at a constant speed. The actual reality is much different, with start / stop and potential low wind velocity situations. Even though the physical dimensions of the bearing and surface finish are the same as rotational speed changes, the required viscosity to maintain Kappa values >1.0 changes as well. As speed increases, the viscosity required to maintain a Kappa value >1.0 decreases. More importantly regarding lubrication of the main shaft bearing, as the speed slows, the required minimum viscosity increases, while there is no immediate change in the bearing temperature. Consider the graphic below in Figure 10 where the columns show the viscosity required to provide adequate lubrication at the indicated rotational speed of the main shaft (primary vertical axis). This is an absolute viscosity required at any temperature based on the bearing rotational speed regardless of bearing temperature. At the highest rotational speed of 19 rpm, on the left, the viscosity required is the lowest (147 cSt). By the same token, the slowest rotational speed of 5 rpm requires the highest viscosity (448 cSt). As the bearing temperature increases, due to load and/or ambient conditions, the viscosity of the fluid in the grease goes down. The red line represents the temperature (in C) at which the installed grease provides the requisite film (secondary vertical axis in Figure 10). Any time the bearing temperature exceeds the red line at the indicated rotational speed, the fluid film of the installed grease is inadequate. - 36 VOLUME 83, NUMBER 2
For example, at 5 rpm, the bearing requires a product with a viscosity of 448 cSt at the operational temperature. The installed grease (red line) can provide a film of 448 cSt only up to a bearing temperature of 23.1 C. The operational implication is that, given a speed of 5 rpm, if the bearing temperature is above 23 C, the Kappa value drops significantly below 1.0 and the bearing is in the distress zone at that speed. This is true for the intended operational speed of the main shaft, where the bearing will be in distress any time the bearing temperature exceeds the ability of the grease to provide the requisite film.
Figure 10 Effect of rotational speed on an applicable, fit for purpose product The base of the red arrow in the modified graphic in Figure 11 indicates that in the best-case scenario, where the main shaft is in steady state and the bearing temperature is within an acceptable range for the installed grease, a decrease in shaft speed from 19 down to 5 rpm pushed the viscosity requirement up, while the bearingâ€™s operating temperature remained unchanged. The fluid film is insufficient at that point (tip of the arrow is significantly above the dashed red line of the installed grease at 5 rpm. The viscosity of the film is ~1/3 of the required, leading to increased metal to metal contact and catastrophic wear.
Figure 11 Effect of changing rotational speed while bearing is in operation, during slow wind velocity - 37 VOLUME 83, NUMBER 2
Contrast that with a synthetic ISO 460 grease that will provide a sufficient film at 40.3 C in the 5 rpm scenario. The dashed green line illustrates the corresponding relationship between bearing temperature and viscosity for a synthetic ISO 460 grease in the same set of circumstances. The gap between the two lines is the temperature window, all along the speed curve, where one product is fit for purpose and the other is not. During low wind velocity conditions, while the bearing temperature was elevated, the film of the installed grease was insufficient to maintain adequate separation of the bearing components. The obvious consequence was that elevated bearing temperatures combined with low wind velocity further placed the bearing in distress. On the other hand, at all speeds from 5 to 19 rpm, and bearing temperatures from 40 to 63 C, an ISO 460 grease would have the requisite film to protect the bearing. The film of the installed grease would be inadequate any time the bearing temperature exceeded 42 C. Another way to view the conditions is to compare Kappa charts where rotational speed and temperature can be varied relative to each other, and the Kappa value is designated by color in Figure 12:
- 38 VOLUME 83, NUMBER 2
Figure 12 Kappa charts for the installed ISO 150 grease (top) and a synthetic, ISO 460 alternative grease as speed and temperature vary On the top is the Kappa chart for the installed grease, and the alternative synthetic, ISO 460 is on the bottom of Figure 12. These charts show the effect of rising bearing operating temperature from 16 (top) to 88 C (bottom) on Kappa. Across the chart from left to right, the rotational speed of the bearing increases from 5 to 20 rpm. The last column is an â€˜average speedâ€™ of 15 rpm. The regions of orange and green indicate adequate bearing lubrication where the Kappa ratio is greater than 1.0. The red is indicative of distress, where Kappa values are less than 1.0. The further down the rotational speed column, the more the Kappa value deviates from the minimum acceptable value of 1.0. This ignores any shock loading during operation, which would increase the surface contact and potential for surface damage. Viewing the main shaft grease selection from a steady-state, best case scenario indicates that the installed grease was fit for purpose only up to 43 C as indicated. Considering the varying wind speed scenario, in conjunction with the historical ambient temperature information, the selection of the ISO 150 grease is cast in an even worse light. - 39 VOLUME 83, NUMBER 2
Operational reality precludes the use of light viscosity products as a means to consolidate products in this case. The resulting bearing damage is evidence that the analysis is accurate. Operational Impact Due to insufficient lubricating film, the bearings were operating a significant portion of the time in a region of the Stribeck curve where surface distress was inevitable. Since the theoretical / projected temperatures were in fact reality, as indicated by the site feedback, the resultant wear would be catastrophic. The wear metals present in the sampled in-service grease confirm the empirical projections and illustrate the extent of the damage experienced by the bearings in operation. The loss of any reserve oxidative resistance would result as the wear metals catalyzed oxidation of the installed grease. These anticipated results have been thoroughly documented. Wear metal results were previously discussed, but the visual inspections of the bearings left no doubt that the site was experiencing serious, catastrophic wear that projected to premature failure of the bearings.
Figure 13 Wear metal scan (left) and visual of centrifuged in-service grease sample (right)
Figure 13 shows data from the analysis of wear metals in a sample of in-service grease. Metallic copper is visible as striations in the centrifuged grease sample. The iron levels exceeded 2.5% of the in-service sample, and the copper was also exceptionally high, indicating significant cage wear. The bulk color of the used grease was black (the fresh grease was beige), illustrating the oxidized condition of the grease. Pressure Differential Scanning Calorimeter (PDSC) testing indicated that the inservice grease had little oxidative life left. Although, it should be noted, because of the high copper, iron and zinc content, these metals may have acted as catalysts during the analysis, possibly increasing the rates of oxidation reactions. In tests at 195 C and 500 psi (ASTM D5483), the induction time for in-service grease was less than 3% of the time for fresh grease.
- 40 VOLUME 83, NUMBER 2
Borescope inspections of selected bearings illustrated the extent of the damage caused by inadequate lubrication of the bearing by the installed grease over time, Figure 14.
Figure 14 Inner race damage visible through borescope inspection of the bearing The projected life of these bearings, under the operational conditions of speed and load is anticipated to be over twenty years where Kappa values are at least 1.0 and routine maintenance is observed (bearing lubricated regularly at appropriate intervals and free of contamination). Bearing manufacturers project bearing life based on loading condition and the capacity / design of the bearing via the life equation: L10 = (C/P) p
Where: L10 is the rated life in hours with 90% reliability C is the basic dynamic load rating (kN) P is the operating equivalent dynamic load (kN) p is the exponent in the life equation (10/3 for roller bearings) Bearing application specific loading and operational information: Radial Load 480 kN Axial Load 120 kN Dynamic Load Rating 5,600 kN Static Load Rating 10,200 kN  Ambient Temperature 0 to 40 C The analog bearing used for the calculations has a dynamic load rating of 5,600 kN and the bearing load as indicated earlier is 480 kN radial and 120 kN axial. The equivalent dynamic load is calculated to be 874 kN via SKF calculation tools.  The load ratio is therefore 6.4 (5,600/874). The L10 in years, assuming adequate lubrication is ~50 years.  The fact that a statistically significant number of the fleet bearings were in failure mode at 9 years set off appropriate alarm bells. Consider the graphic in Figure 15:
- 41 VOLUME 83, NUMBER 2
Figure 15 Theoretical bearing life, assuming adequate lubrication at 19 rpm versus bearing operating temperature As stated previously, when bearing temperatures are at or below 42 C, the theoretical bearing life far exceeds the 20-year target (175,000 operational hours). However, the actual bearing temperatures based on historic weather data for the installation region significantly impacts the bearing life. In contrast, an ISO 460 synthetic grease would provide the same life expectancy at much higher bearing operational temperatures, up to 63 C. Based on SKF calculation methodology, where the minimum required viscosity is slightly lower, the relative difference in bearing life expectancy is significant, with the installed grease only supporting a theoretical life that is ~25% of the theoretical life with an appropriate ISO 460 grease at a bearing temperature of 60 C.
Figure 16 SKF calculated evaluation of the bearing under the same conditions, illustrating a mirror response of negative bearing life impact as temperatures rise - 42 VOLUME 83, NUMBER 2
Recall that historical weather for the region projected high bearing temperatures to be over 50C at least 33% of the time, and 56% of the time the bearings will exceed the distress point of the installed grease. If it was just as simple as the bearing responding to the ambient temperature changes, the effect on the bearing distress point could be minimized. However, the bearing temperature does not cool immediately, and the nacelle ambient often exceeds the outside ambient, reducing the delta T that could drive the heat transfer away from the bearing. If you consider the impact of variable speed on the viscosity required, as discussed earlier, the impact is potentially more dramatic. Compounding the effects of temperature is the presence of wear metals in the bearing and grease itself. The wear metal particles oxidize the grease, but also can be large enough to bridge the already thin fluid film and cause point loading and fatigue in the bearing. This would compound the detrimental effect on the bearing performance and anticipated life. In this case, main shaft bearings are manually lubricated twice per year, and the supply of fresh grease is not sufficient to flush away the wear particles and spent grease. Catastrophic failure is not a question of if, but merely how long before the bearing condition reaches the ‘point of no return’. The
wearing away of the surfaces in the cage and assembly allows the bearing to shift axially in the housing as well, which causes more mechanical faults and heat, further exacerbating the conditions and hastening the impending failures.
Mitigation and Recommendations The initial decisions have had a slow, progressive negative effect on the performance of the fleet. However, the pace of the bearing failure increases with all the mitigating and compounding
More Than Just a Drop in the Bucket
VANDERBILT CHEMICALS, LLC CERTIFIED TO ISO 9001:2015 10002461
MOLYVAN® 855 Friction Reducer
Today’s high performance lubricants require special additives to perform successfully. MOLYVAN® 855 is an organo-molybdenum additive that contains no phosphorus or sulfur and is more cost effective than traditional molybdenum dithiocarbamates. Lubricants formulated with MOLYVAN® 855 exhibit enhanced oxidation and wear protection, as well as reduced timing chain wear and improved low speed pre-ignition (LSPI) performance, two new requirements proposed for GF-6. Order a sample and discover the many benefits of this unique additive component in your lubricant formulation.
email@example.com www.vanderbiltchemicals.com (203) 853-1400 30 Winfield Street, P.O. Box 5150, Norwalk, CT 06856-5150, USA Registered and pending trademarks appearing in these materials are those of R.T. Vanderbilt Holding Company, Inc. or its respective wholly owned subsidiaries. For complete listings, please visit this location for trademarks, www.rtvanderbiltholding.com.
- 43 VOLUME 83, NUMBER 2
circumstances that are a result of the initial decision to apply a grease that was not fit for the operational conditions. The damage cannot be reversed, only mitigated using a fit for purpose grease that will minimize further wear through proper viscosity / adequate fluid film. The grease selection must first address the viscosity of the film at the anticipated ambient and corresponding bearing temperatures. There is simply no substitute for providing a lubricating grease that can provide adequate fluid film thickness at the highest anticipated temperature (or at least the clear majority of the operational time). This must be balanced with the minimization of low temperature torque and lost bearing efficiency during the coldest ambient conditions. Fleet operations management must evaluate the state of the fleet and prioritize the actions to mitigate the operational and financial impact. The economic impact of replacing one of the fleet main shaft bearings is approximately $300,000. The replacement of a bearing involves a loss of operational revenue, and a substantial health and safety risk to the workers tasked to install the new bearing. The wholesale replacement of the main shaft bearings across this farm would exceed $40MM. Fleet-wide bearing replacement is exceedingly expensive, and therefore it is prudent to perform â€˜bearing triageâ€™. Bearing triage involves additional costs for analytical evaluation of the in-service grease and bearings. It also involves inspection costs above and beyond anticipated maintenance and operations budgets. These services also come with inherent health and safety concerns. The bearing replacements can be prioritized by the aggregate of loss of mechanical tolerances in the turbine drive train (the bearing is only part of the equation), the level and identity of wear metals present in sampled grease, and operational bearing temperature relative to the ambient conditions at site. The wholesale change of the installed grease is the starting point. Close monitoring of the bearing assets after the change can further guide the site management on priorities regarding bearing replacement. Conclusions As more newly installed electrical generation capacity is supplied by wind turbine fleets, the asset health of critical path components of these fleets should be prioritized over convenience and simplification by OEMs and operational staff. Blade and main shaft bearings have some common lubrication needs, but their primary failure modes diverge. The formulary methods for addressing the diverging failure modes of the bearings in question are different enough to require careful consideration regarding grease selection for the applications. The most appropriate grease for each bearing application, most likely, will not be the same. Grease selection, without careful consideration of the operational realities of bearing temperature and rotational speed, can lead to catastrophic, expensive failures and mitigation costs. The fact that the effects of grease selection are not immediately evident conceals the true cost and delays the expensive remediation expenses that then become the responsibility of the owner/ operator of the fleet. Most likely, the consequences of these decisions will materialize long after the warranty or service contract expires, leaving the owner responsible to absorb these unnecessary and avoidable expenses, along with loss of operating revenue and increased health and safety risks incurred to make the necessary repairs. Paramount in the grease selection process should be viscosity at the anticipated operating temperature of the bearing. However, greases are complex systems of base oils, performance enhancing additives and thickeners. These components play an important role in the ultimate performance of the chosen product in the specific application. Understanding the application needs and overlaying the performance of candidate greases in efforts to mitigate failure modes is the secondary step in the process. - 44 VOLUME 83, NUMBER 2
Asset health and reliability of the turbine should be placed ahead of any compromise on product selection. Grease selection should be based on available data, not conjecture, anecdotal stories and hope. Industry available tools can accurately predict lubrication related outcomes as illustrated by this case study. These tools are based on empirically developed data, backed by years of field validation and the collective experience of professionals in the bearing and lubrication industry. When compromises are made, the industry established calculation models predict bearing distress in the application. The long-term, real-world outcome verifies the calculations. Compromise is accompanied by an associated cost. In this case the costs and risks proved to be too high. References  Federal Energy Regulatory Commision (FERC), “Energy Infrastructure Update Report,” Federal Energy Regulatory Commision (FERC), 2018.  American Wind Energy Association, American Wind Energy Association, 2017.  U. S. E. I. Administration, “Monthly Energy Review,” April 2017.  SKF , SKF General Catalog- 5000E, Media-Print, June 2003.  A. Yano, Y. Noda, Y. Akiyama, “Evaluation of Fretting Protrection Property of Lubricating Grease Applied to Thrust Bearing,” Tribology Online- Japanese Society of Tribologists, vol. 5, pp. 52-59, February 2010.  C. Schwarze, Modified Riffel: Institute for Tribology and Energy Conversion Machines iTR-Riffel-Test, 2011.  A. Jacobs, iME- Rothe Erde Riffel Test: iME Institue fur Maschinenelemente und Maschinenggestaltung, 2002.  SKF, “http://webtools3.skf.com/BearingCalc,” 2018. [Online]. [Accessed 2017].
- 45 VOLUME 83, NUMBER 2
An Interview with Mr. Durgesh Sanjivrao Chandavarkar By Raj Shah and Mary Moon April 26, 2019 pounds! Karnataka and Goa are historic places with many ancient churches and temples. My experience growing up there is the reason that I still love nature and water. NLGI: What was your first position at Standard Greases? How did your career develop? Mr. Durgesh Sanjivrao Chandavarkar is Chairman & Managing Director of Standard Greases & Specialities Pvt Ltd (SGSPL), one of the largest lubricating grease manufacturers in Asia, with headquarters located in Mumbai, India. Mr. Chandavarkar has served as an officer & a leader of the India Chapter of NLGI since its founding in 1997. He graciously shared his time & views with NLGI about his career, his Company, the Grease Industry, & (of course) his favourite food & companions for ‘a dinner to dream about’.
DSC: I am basically a marketing man. In 1992, I was asked to lead Standard Greases based on my marketing experience and leadership qualities. Since I joined the Company, I have worked closely with Mr. Vinod Vyas, who founded Standard Greases in 1983. The graph of the Company’s results has continued to grow upwards. Standard Greases today is the largest private label grease manufacturer in India. Under my leadership, the Company has diversified in many ways. We decided to pursue
backward integration. In 1995, we set up a plant, Royal Castor Products Ltd, to manufacture hydrogenated Castor Oil (HCO), 12-Hydroxy Stearic Acid (12HSA), and other Castor Oil Derivatives. HCO and 12-HSA are major raw materials needed for grease manufacturing. Our Plant, co-owned with a Japanese equity partner, is located at Sidhpur in the Indian state of Gujarat, which is a hub of castor oil production. At present, Standard Greases has three grease manufacturing plants with a total capacity of 42,000 MTs and two oil blending plants with total capacity of 120,000 KL. All of these plants are certified ISO 9001:2015, ISO 14001:2015, ISO 18001:2007, and TS 16949:2009. Over 10% of our products are exported to various countries. We have our own ‘SG Transport’ with a fleet of more than 60 tankers for liquid transportation.
NLGI: Please tell us a little bit about where you grew up. DSC: I was brought up in one of the most beautiful places on the southwest coast of India. I grew up near the city of Karwar in the state of Karnataka, and the neighbouring state of Goa. This place is full of serene beaches and lush green gardens with many coconut, mango, and jackfruit trees. The jackfruit is the largest fruit that grows on trees; one fruit can weigh as much as 55 kg or over 100
Standard Greases & Specialities Pvt Ltd is one of the largest lubricating grease manufacturers in Asia. - 46 VOLUME 83, NUMBER 2
To keep pace with the latest developments in the field of lubrication, we have a full fledged state of the art R&D Centre equipped with the latest testing facilities. The R&D Centre is recognised by the Government of India. Additionally, we have a unique pilot plant in the city of Silvassa, an industrial hub located in the Union Territory of Dadra and Nagar Haveli on the northwest coast of India. NLGI: What were some key decisions that helped Standard Greases grow and become the #1 private label grease producer in India? DSC: From the very beginning, Standard Greases adopted certain policies that helped it grow at a faster rate than competitors. Standard Greases has become one of the largest grease manufacturers in the Asia Pacific region. First, despite having enough technical and commercial capabilities to develop our own lubricant brands, we decided not to do so because that would lead us to compete with our own customers. This policy has given our customers added confidence in us. We have over 20 customers including the reputed MNCs. The technical information, formulations, etc. of each customer is not shared with anybody and is kept confidential. Secondly, the quality of the products and services are top most priorities in our system
Inside one of Standard Greases’ plants for grease production
without any compromise. We have been able to retain our customers for more than three decades. NLGI: Standard Grease is growing its business in India and expanding worldwide. What are your greatest challenges in leading this growth? DSC: The Indian market is almost matured and a price sensitive market. The recent growth of many small scale grease manufacturers has led to tough competition in the grease market. It is a real challenge to sustain the Company’s growth under such circumstances. So we need to develop innovative, new, more economical, and better products for our customers. With our modern R&D Centre, we are able to develop high performance products as per our customers’ requirements.
NLGI: What do you think about the position of India in the global grease industry? What are your thoughts about the future of the grease industry in India? DSC: India is the third largest grease consumer in the world after China and North America. With its growing economy, the Indian market is expected to grow at a CAGR or compound annual growth rate between 1 and 1.5 % in the next five years. The Indian market is also maturing, and it is predicted that the demand for high performance greases will grow, especially in the automotive and industrial sectors. Over 90% of the greases produced in India are based on lithium or lithium complex soaps. India imports large quantities of Lithium Hydroxide, and its price is highly volatile. The availability
The full fledged state of the art R&D Centre at Standard Greases - 47 VOLUME 83, NUMBER 2
of Lithium Hydroxide is also sometimes a major constraint. It is high time that we should look for alternatives to lithium base greases. There are several options available that can be explored. The alternatives are polyurea greases, aluminium complex greases, calcium sulphonate complex greases, etc. Depending on the applications, suitable greases can be selected. Looking at the future grease market, another important field is specialty greases. Specialty greases such as thermal greases, nano greases, greases for electrical vehicles, etc. should be explored. The Indian government is pushing the introduction of electric vehicles in the next two to three years to reduce pollution, which is a major concern in some of our metro cities. However, the introduction of EVs will not lead to a drop in grease demand. NLGI: What are your thoughts about the future of the grease industry around the world? DSC: Over recent years, there has been no major breakthrough in grease technology. We have been using the same types of thickeners and base oils with only slight variations. Some innovations are taking place in additive technology; however, these are yet to be established. Efforts must be made to develop innovative new thickeners and new base oils that can withstand the severe operating conditions experienced by lubricants in modern machines.
We also need to emphasise and concentrate on developing biodegradable lubricants. In this context, our sister concern, Royal Castor Products Ltd., has developed bio-based lubricants that will be of great interest to the industry. NLGI: How would you describe your management style? DSC: I believe in giving full responsibility to the people working with me and guiding them as and when required. I love to interact with the people in my organization right from the bottom all the way to the top. People form an important part of any organization.
Leaders should be able to take on work assigned to the managers. They should be innovative and passionate about their work. Leaders should have good decision making capabilities. A good leader will always develop his deputies to take over in future. NLGI: Did particular people influence your career? DSC: Working in the grease industry, I have come across many prominent professionals such as Dr. Bhatnagar, Dr. Malhotra, Dr. Ramkumar, Dr. Anoop Kumar and Dr. Raj Shah who have enriched my knowledge about the grease industry.
NLGI: Do you have any advice for people who might want to become managers or leaders?
NLGI: You are a leader of NLGIIndia Chapter. How did you get involved in NLGI-IC?
DSC: Managers must be committed to their work. They should be able to take up their responsibility and be fully focused.
DSC: I have been involved in NLGI-IC activities from its very beginning. NLGI-IC was founded in 1997 by Dr. Akhilesh Kumar Bhatnagar, former Director R&D
Chandavarkar, Bhatnagar, and V. N. Sharma with delegates at an NLGI conference - 48 VOLUME 83, NUMBER 2
of Indian Oil Corporation Ltd. and the late Dr. Chandrashekhar, CMD of Balmer Lawrie & Co. Ltd. I was also a founder and held the Sr. Vice President of NLGI-IC position for many years. I was recently the President for two years, from 2017 to 2019. NLGI: How does NLGI-IC contribute to the grease industry? DSC: NLGI-India Chapter holds its conferences every year beginning with its first conference at Nainital in 1999. Over the years, the participation of the grease industry and other allied industries in these conferences has increased. Large numbers of foreign delegates also attend these conferences, which are held at exotic cities of India. The technical papers presented are of high standards. The conferences also conduct various cultural programmes highlighting the culture of different regions of India, and these cultural programmes have become very popular.
Dr. Raj Shah, Koehler Instrument Company congratulating Dr. Chandavarkar and his team on completion of another wonderfully run NLGI India Conference - 49 VOLUME 83, NUMBER 2
NLGI-IC also conducts educational courses about lubrication every year. So far, we have conducted 21 educational courses about lubricants for industries such as the Cement Industry, Steel Industry, Textile Industry, Automotive Industry, etc. The response to such educational programmes is very encouraging, and participation in these courses is growing over the years. Our courses give good knowledge about greases and also help engineers in understanding and solving the problems faced by their industry. We have also conducted five Round Robin Tests with laboratories. NLGI-IC also publishes Grease Tech India, a technical journal for the grease industry.
Chandavarkar and Vyas with delegates
NLGI: What are some of NLGIIC’s plans for the future?
contribute to the growth of grease industry.
DSC: NLGI-IC looks forward to increasing participation in their conferences from countries like Malaysia, Thailand, Singapore, Philippines, etc. where the consumption of lubricating grease is growing. We would like to take up the leadership role and involve these South Asian countries to participate and
NLGI India also plans to start research projects in lubricating greases in association with universities and research organizations.
Petro-Lubricant Testing Laboratories, Inc.
NLGI: Do you have time to be involved in other volunteer activities?
116 Sunset Inn Road Lafayette, N.J. 07848 Phone: 973-579-3448 Email: Info@petrolube.com
•Over 600 Standardized, Custom and Industry Test Methods (ASTM, Fed. Std. 791, DIN, PTI, ISO, SAE, EN, IP, JIS, AAR etc. and Many Corporate Specifications)
•Affordable RUSH Testing Fees
•Upfront Pricing and Quotes Available
•Immediate Access to Knowledgeable Staff •38 Years of Experience Testing Lubricants of All Types
Quality Assurance and Certifications: ISO 9001-2015 - ISO/IEC 17025-2017 - 50 VOLUME 83, NUMBER 2
DSC: I am a firm believer that you must contribute something for your society. So I regularly donate to educational institutes for the poor students. I also help some organizations that work to help mentally challenged children.
Satellite Launch Vehicle (PSLV) and successfully flight testing a GSLV (Geosynchronous Satellite Launch Vehicle, an expendable launch system). He has been conferred with the Padma Shri, Padma Bhushan, and Padma Vibhushan awards besides several other awards for his contributions to Indian Space Research. He
Kasturirangan addresses delegates at a meeting of NLGI-IC
NLGI: When you are not working, where is your favorite place to travel? DSC: I am a nature-loving person, and I enjoy being with nature. My favourite place to travel is New Zealand. NLGI: If you could have dinner with any three people, living or deceased, who would they be and why? And what might be on the menu? DSC: I would love to have dinner with three friends because during our interactions I have learnt a lot, & I have great love and respect for them. First, there would be my friend, philosopher, and guide, Dr. Krishnaswamy Kasturirangan. He was the chairman of the Indian Space and Research Organization (ISRO). Under his leadership, Indiaâ€™s space programme achieved several major milestones such as successfully launching the Polar
Servo Filling Systems
- 51 VOLUME 83, NUMBER 2
is on the governing council of the Raman Research Institute. He was also a member of the Planning Commission and member of Raj Sabha. As a Chief Guest, he chaired the NLGI-India Conference in Goa in 2000. Besides being a great scientist and a great leader, Dr.
Kasturirangan is great human being and my role model. During meetings with Dr. Kasturirangan, I learnt many things from him that helped me evolve as a better person. Dr. Kasturirangan shared his thoughts with NLGI: “My association with Mr. Durgesh Chandavarkar goes back to nearly two decades. This period to me has been very eventful, as I had the good fortune of seeing him scaling the multidimensional
ladder of life which includes, besides his core business interest, deep commitment to social upliftment, extraordinary display of philanthropy and above all caring & inspiring all those like me who came in contact with him in different contexts. I have never experienced an instance when he compromised the core values of his life over this long period of knowing him. He will always have a special place in my heart; a great source of strength and courage which I can always draw upon in times of need.”
Another person with whom I would love to dine is the late Shri N. Raghunathan, IAS (Indian Administrative Service), former Defence Production Secretary, Government of India, & Chief Secretary, Government of Maharashtra. My third choice would be the late Shri S. Prabhakaran, IAS, former Secretary, Power, Government of India, & also Principal Secretary, Government of Maharashtra. We all love South Indian vegetarian dishes, which would be the main course of our dinner menu.
Industry Calendar of Events 2019 Please contact Denise if there are meetings/conventions you’d like to add to our Industry Calendar, firstname.lastname@example.org (Your company does not have to be an NLGI membeer to post calendar items.)
June 8 - 11, 2019 86th NLGI Annual Meeting JW Marriott Las Vegas
September 21-24, 2019 ILMA Annual Meeting The Broadmoor, Colorado Springs, CO
Advertiser’s Index Frigmaires Engineers, page 27 Patterson Industries Canada - A Division of All-Weld Company Limited, page 9 Petro-Lubricant Testing Labs, page 50 ProSys Servo Filling Systems, page 51 Vanderbilt Chemicals, LLC, page 43 Zschimmer & Schwarz USA, page 49
- 52 VOLUME 83, NUMBER 2
Fundamental study of the initial agglomeration of lithium soap thickener in lubricating oil Report March 2019 Paul Shiller1, Nikhil Prasad1, and Gary Doll1 1 The University of Akron 1 Introduction This is an update of the progress of the project which started August 2018. There are two parts to this project • The ﬁrst is to physically manufacture soap thickened grease at the initial point of thickener agglomer-ation. – The initial point of thickener agglomeration is the critical micelle concentration. – For the Li-12hydroxy stearate thickener grease that concentration is between 3% and 5% soap concentration. • The second is to model the thickener agglomeration. – Modeling will initially consist of determining the attractive or repulsive force between thickener molecules. – After the forces are determined a molecular dynamics simulation will be constructed to match the results of testing the physical grease 2 Current Work Grease was formulated in the lab by mixing lithium hydroxide and 12-hydroxy stearic acid in an ISO VG 10 base oil. • Multiple batches with concentrations of 3%, 4%, and 5% soap were formulated, see the appendix for procedure and recipe. – Moisture testing was performed to determine the end point of the reaction. – Cone on plate rheological testing was performed to determine if the critical micelle concentration was reached. * The determining factor is the relative position of the storage and loss moduli in the plateau region of an oscillating stress sweep rheology experiment. * If the storage modulus is above the loss modulus the thickener has formed. If the storage modulus is below the loss modulus the thickener has not formed yet. – Dynamic light scattering experiments were performed to determine the shapes and orientation of the agglomerates. * Results are inconclusive at this time due to the opaque nature of the mixtures Thickener agglomeration modeling was started by calculating energies of interaction between thickener molecules • Modeling was started by establishing the orientation of the Li-12hydroxystearate molecules relative to each other. – A semi-empirical method with a two body repulsion force was chosen to determine the interaction forces and energies – Initial calculations show a small van der Waals attraction between two Li-12hydroxystearate molecules. - 53 VOLUME 83, NUMBER 2
• Initial setup of the molecular dynamics calculations are in progress. – The system, is being setup now, consists of a 60 A cube with 14 Li-12hydroxystearate molecules and 197 hexatricontane (36 carbon oleﬁn) molecules. 3 Highlights Two results of the project so far are given here. The rheological testing results are unexpected but seem an important step in the thickener agglomeration process. The calculation results show that there is some force that can hold the agglomerates together. Figure 1 below shows measurements of the cone on plate oscillating stress sweep experiment of 4% and 5%soap concentration. This was plotted with an x-axis of % strain. The 5% concentration shows normal grease response. The 4% shows a gap in the response going from about 10% strain to over 1000% strain with a small increase in stress. The agglomerates have been disrupted. The force necessary to disrupt the agglomeration process here is about 200 Pa to 300 Pa. In the low stress plateau region the storage modulus is greater than the loss modulus so there are viscoelastic materials; i.e. grease.
Figure 1: Cone on plate oscillating stress sweep experiment method results of 4% (right ﬁgure) and 5% (left ﬁgure) soap concentration greases. Plotted with x-axis of % strain.
- 54 VOLUME 83, NUMBER 2
4 Next steps Grease formulation: • Continue cone on plate rheology. – Get a more precise value for the force needed to disrupt the thickener agglomerates. – Perform frequency sweep experiments to determine relaxation times for molecular movement. • Modify method to enable dynamic light scattering measurements to be obtained. Agglomerate modeling: • Calculate van der Waals interaction along more orientation parameters. • Begin molecular dynamics calculations.
Figure 2: Orientation of two thickener molecules in space.
Figure 3: Energy vesus separation in the z-direction and ﬁt to Lennard-Jones 6-12 potential.
References  J. E. Lennard-Jones and S. Chapman. On the determination of molecular ﬁelds. —ii. from the equation of state of a gas. Proceedings of the Royal Society of London. Series A, 106, October 1924. - 55 VOLUME 83, NUMBER 2